Thermal shock occurs when a thermal gradient causes different parts of an object to expand by different amounts. This differential expansion can be understood in terms of stress or of strain, equivalently. At some point, this stress can exceed the strength of the material, causing a crack to form. If nothing stops this crack from propagating through the material, it will cause the object's structure to fail.
Failure due to thermal shock can be prevented by;
- Reducing the thermal gradient seen by the object, by changing its temperature more slowly or increasing the material's thermal conductivity
- Reducing the material's coefficient of thermal expansion
- Increasing its strength
- Introducing built-in compressive stress, as for example in tempered glass
- Decreasing its Young's modulus
- Increasing its toughness, by crack tip blunting (i.e., plasticity or phase transformation) or crack deflection
Effect on materialsEdit
Borosilicate glass is made to withstand thermal shock better than most other glass through a combination of reduced expansion coefficient and greater strength, though fused quartz outperforms it in both these respects. Some glass-ceramic materials (mostly in the lithium aluminosilicate (LAS) system) include a controlled proportion of material with a negative expansion coefficient, so that the overall coefficient can be reduced to almost exactly zero over a reasonably wide range of temperatures.
Reinforced carbon-carbon is extremely resistant to thermal shock, due to graphite's extremely high thermal conductivity and low expansion coefficient, the high strength of carbon fiber, and a reasonable ability to deflect cracks within the structure.
To measure thermal shock, the impulse excitation technique proved to be a useful tool. It can be used to measure Young's modulus, Shear modulus, Poisson's ratio and damping coefficient in a non destructive way. The same test-piece can be measured after different thermal shock cycles and this way the deterioration in physical properties can be mapped out.
Relative robustness of materialsEdit
Thermal shock parameter in the physics of solid-state lasersEdit
The laser gain medium generates heat. This heat is drained through the heat sink. The transfer of heat occurs at a certain temperature gradient. The non-uniform thermal expansion of a bulk material causes the stress and tension, which may break the device even at a slow change of temperature. (for example, continuous-wave operation). This phenomenon is also called thermal shock. The robustness of a laser material to the thermal shock is characterized by the thermal shock parameter. (see above)
Roughly, at the efficient operation of laser, the power of heat generated in the gain medium is proportional to the output power of the laser, and the coefficient of proportionality can be interpreted as heat generation parameter; then, The heat generation parameter is basically determined by the quantum defect of the laser action, and one can estimate , where and are frequency of the pump and that of the lasing.
Then, for the layer of the gain medium placed at the heat sink, the maximal power can be estimated as
where is thickness of the layer and is the transversal size. This estimate assumes the unilateral heat drain, as it takes place in the active mirrors. For the double-side sink, the coefficient 4 should be applied.
The estimate above is not the only parameter which determines the limit of overheating of a gain medium. The maximal raise of temperature, at which the medium still can efficiently lase, is also the important property of the laser material. This overheating limits the maximal power with an estimate
Combination of the two estimates above of the maximal power gives the estimate
is thermal loading; parameter, which is important property of the laser material. The thermal loading, saturation intensity and the loss determine the limit of power scaling of the disk lasers . Roughly, the maximal power at the optimised sizes and , is of order of . This estimate is very sensitive to the loss . However, the same expression can be interpreted as a robust estimate of the upper bound of the loss required for the desired output power :
All the disk lasers reported work at the round-trip loss below this estimate. The thermal shock parameter and the loading depend on the temperature of the heat sink. Certain hopes are related with a laser, operating at cryogenic temperatures. The corresponding Increase of the thermal shock parameter would allow to soften requirements for the round-trip loss of the disk laser at the power scaling.
Thermal shock testingEdit
Thermal shock testing exposes products to alternating low and high temperatures to accelerate failures caused by temperature cycles or thermal shocks during normal use. The transition between temperature extremes occurs very rapidly, greater than 15 °C per minute.
Equipment with single or multiple chambers is typically used to perform thermal shock testing. When using single chamber thermal shock equipment, the products remain in one chamber and the chamber air temperature is rapidly cooled and heated. Some equipment uses separate hot and cold chambers with an elevator mechanism that transports the products between two or more chambers.
Glass containers can be sensitive to sudden changes in temperature. One method of testing involves rapid movement from cold to hot water baths, and back.
Examples of thermal shock failureEdit
This section does not cite any sources. (June 2013) (Learn how and when to remove this template message)
- Hard rocks containing ore veins such as quartzite were formerly broken down using fire-setting, which involved heating the rock face with a wood fire, then quenching with water to induce crack growth. It is described by Diodorus Siculus in Egyptian gold mines, Pliny the Elder, and Georg Agricola.
- Ice cubes placed in a glass of warm water crack by thermal shock as the exterior surface increases in temperature much faster than the interior. The outer layer expands as it warms, while the interior remains largely unchanged. This rapid change in volume between different layers creates stresses in the ice that build until the force exceeds the strength of the ice, and a crack forms, sometimes with enough force to shoot ice shards out of the container.
- Incandescent bulbs that have been running for a while have a very hot surface. Splashing cold water on them can cause the glass to shatter due to thermal shock, and the bulb to implode.
- An antique cast iron cookstove is a simple iron box on legs, with a cast iron top. A wood or coal fire is built inside the box and food is cooked on the top outer surface of the box, like a griddle. If a fire is built too hot, and then the stove is cooled by pouring water on the top surface, it will crack due to thermal shock.
- It is widely hypothesized [by whom?] that following the casting of the Liberty Bell, it was allowed to cool too quickly which weakened the integrity of the bell and resulted in a large crack along the side of it the first time it was rung. Similarly, the strong gradient of temperature (due to the dousing of a fire with water) is believed to cause the breakage of the third Tsar Bell.
- Thermal shock is a primary contributor to head gasket failure in internal combustion engines.
- US Patent 6066585, "Ceramics having negative coefficient of thermal expansion, method of making such ceramics, and parts made from such ceramics", issued 2000-05-23, assigned to Emerson Electric Co.
- T. J. Lue; N. A. Fleck (1998). "The Thermal Shock Resistance of Solids" (PDF). Acta Materialia. 46 (13): 4755–4768.
- W.F.Krupke; M.D. Shinn; J.E. Marion; J.A. Caird; S.E. Stokowski (1986). "Spectroscopic, optical, and thermomechanical properties of neodymium- and chromium-doped gadolinium scandium gallium garnet" (abstract). JOSA B. 3 (1): 102–114. Bibcode:1986JOSAB...3..102K. doi:10.1364/JOSAB.3.000102.
- D.Kouznetsov; J.-F.Bisson (2008). "Role of the undoped cap in the scaling of a thin disk laser". JOSA B. 25 (3): 338–345. Bibcode:2008JOSAB..25..338K. doi:10.1364/JOSAB.25.000338.
- D. Kouznetsov; J.F. Bisson; J. Dong; K. Ueda (2006). "Surface loss limit of the power scaling of a thin-disk laser" (abstract). JOSA B. 23 (6): 1074–1082. Bibcode:2006JOSAB..23.1074K. doi:10.1364/JOSAB.23.001074. Retrieved 2007-01-26.; [permanent dead link]
- ASTM C149 — Standard Test Method for Thermal Shock Resistance of Glass Containers